Presentation on theme: "Session 504: Intro to Marine Composites Design-Advanced Methods Dr. Paul H. Miller, PE U. S. Naval Academy."— Presentation transcript:
Session 504: Intro to Marine Composites Design-Advanced Methods Dr. Paul H. Miller, PE U. S. Naval Academy
Intro to the Advanced! Goals: –Advanced methods for marine composites design (Session 404 was basic methods) –Some “lessons learned the hard way” (also called “case studies”) –Some entertainment value!
My assumptions! You have some background in composites fabrication and design –You know what the common fibers and resins are (E-glass, epoxy, etc.) –You know the basic English units of length, force, area, time –You have used “scantling rules” such as ABS, ISO, Herreshoff, etc.! –You have designed using metal.
What is “design”? The purposeful arrangement of parts To create in a highly skilled manner A drawing or sketch
What is “Marine Composites Design”? Intelligent selection and combination of materials (resins, fibers, cores) to create a structure that fulfills a customer’s requirements Communicating that information!
This Seminar’s Focus Demonstrating advanced analysis methods Some information on selecting materials
General Design Approaches Numerical methods (number crunching) Experimentation (prototypes) Empirical development (small changes each time) Plagiarism! (Not recommended if you are in college) Also called, “benchmarking”.
Numerical Structural Design Requires: 1.Geometry (what will the part look like, dimensions of length, width, maybe thickness) 2.Loads 3.Material properties, and 4.An analysis method (what theory to use)
The Most Fun Part is: Figuring out what it will look like! –In general, smaller parts require less structure, but also require more tooling costs and labor costs –Joints are expensive! –Aim for few parts
The Hardest Part is: What are the loads? Brainstorm on all the reasonable ways your customers can abuse your product! Did you think about high heels?
Easier Methods from Session 404 Combined methods (loads and analysis). Often called “Scantling Rules” American Bureau of Shipping (ABS) Lloyds, DnV, ISO, etc. Gerr’s Elements of Boat Strength Herreshoff’s, etc.
Advanced Methods in this Seminar Loads calculated independently from structural theory CFD, LPT, CLT, FEA, TLA, etc. Potentially more accurate, so potentially lighter and less expensive –break even point?
Material Properties For preliminary analysis only you can get properties from Greene or Scott. For detailed design it is usually not worth the effort of advanced analysis methods if you don’t know the actual laminate properties
Scott Tables Example Fig 11 For a 45% resin content, all woven laminate typical of very good hand layup, tensile strength is 36000 psi 36 55 Only for typical mat, cloth and woven roving with polyester (conservative for other resins)
Greene Tables Appendix A Example –SCRIMP 7781/epoxy –34% resin content –Tensile strength is 56000 psi! www.marinecomposites.com Free download!
Testing Rules of Thumb Choose tests most appropriate to your application. Greene has good summary of common tests ASTM D3039 Test for tensile strength and modulus
Finding Laminate Properties Not in Scott Other than testing, the best method is Classical Lamination Theory (CLT). It is also called Laminate Plate Theory. It is nothing more than matrix math and can be done on a spreadsheet. Shareware programs are nice as they include features like material libraries
Example: We have a laminate that is three plies of 24 oz woven roving at 0/90, 0/90, 0/90, but it twists too much, so we want to know its properties if the middle ply is rotated 45 degrees Get 0/90 props from Scott Et=1.95 msi, Ec= 2.2 msi, ten str. = 29 ksi, comp str = 26 ksi, shear str. = 11 ksi, shear mod = ?, poisson’s = ?
New tensile strength is: 2.88 x 1000 /0.111 =25,950 psi
New shear strength is: 1.38 x 1000 /0.111 =12,432 psi
CLT/LPT Great way to find material properties for various combinations of mat, cloth, woven roving, uni, etc. Is used in composite elements in finite element analysis!
FEA Geometric modeler that internally generates equilibrium equations for force and displacement Steep learning curve, but great results Best for performance applications where stiffness or weight is critical
A Case Study A 77-foot performance cruiser designed by Carl Schumacher
FEA work Designer subcontracted out structural FEA design Designer provided dxf files for all geometries (hull, appendages) FEA consultants optimized and specified construction Designer did hull structure drawings Consultants did keel structure drawings and interfaced with keel and hull manufacturer to ease construction Consultants took 323 manhours, reduced structural weight 28%.
Design Limit Load Cases Upwind in heavy air, wave height equal to freeboard, wave length equal to boat length Slamming (from CFD consultant) Grounding (to ABS loads!) Lifting Each load case drove the design of different parts of the boat.
Upwind in 30 knots on port tack Rig loads supplied by mast maker
Displacements (25x) Maximum displacement = 3.32” Max rotation 0.5 degrees
Factors of Safety Tsai-Wu or Max Stress or Hashin Minimum “real” FOS = 2.25 Not “real”!
Session 206: Grounded! Speed was 30% higher than ABS Assumption!
Hull Damage Outer Ply Factor of Safety Correlation better than 95%!
FEA Suggestions A great tool to evaluate unintentional and planned modifications Efficient if performance is an issue or is a simple case (some projects less than 1 hour) Practice makes perfect Must use composite elements!
Final Thoughts Advanced marine composites design uses LPT and FEA more and more every day due to their demonstrated advantages Some engineering background is needed for the former, more for the latter! The Three Wright Brothers! Sleipner!